molecular dynamics simulation of synthetic polymers molecular dynamics simulation of synthetic...
Post on 24-May-2020
Embed Size (px)
Molecular Dynamics Simulation of Synthetic Polymers
Claudia Sandoval Center for Bioinformatics and Integrative Biology (CBIB), Facultad de Ciencias Biológicas
Universidad Andres Bello, Santiago Fraunhofer Chile Research Foundation - Center for Systems Biotechnology, FCR-CSB
The polymeric systems are great interesting both academic and industrial level, due to interesting applications in several areas. Nowadays, the trends for the development of new materials are focused on the study of macromolecular complex systems. A macromolecular complex system is formed by the interaction between the macromolecules of the same system. There are many macromolecular complex systems; this chapter will refer to complex systems of synthetic polymer blends(Donald R. P., 2000) and synthetic polymer at the air- water interface(Gargallo et al., 2011). The most synthetic polymers are characterized by flexible structure able to adopt multiple and variable forms. The study about molecular behavior in polymers has attracted the attention of many researchers over the years. Studies in dilute solutions of macromolecules have contributed to solving the problem relating to the molecular characterization. Despite, the emergence of characterization methods and theories that have allowed for interpretation of experimental behavior, researchers still have not fully resolved the problem with interactions at the atomic level in polymer systems. The most polymers are amorphous so in some cases are impossible to obtain information about atomic structure through x-ray techniques or atomic force microscopy. At this point, the computer simulations have played an important role in microscopic understanding of dynamical properties of some polymeric systems.
In this chapter a review of molecular simulation methodologies focused on polymer systems will be discussed. This review is based on two case studies. The first one corresponds to a monolayer of amphiphilic polymers and their study at the air-water interface(Gargallo et al., 2009). Three polymers were selected Poly(ethylene oxide) (PEO), Poly(tetrahydrofuran) (PTHF) and Poly(-caprolactone) (PEC) and their cyclodextrin inclusion complexes. The second system corresponds to study the motion of side chains of polymers in condensed phase. For this reason, a diblock copolymers of Polystyrene-block-poly(t-butylacrylate) has been considered(Encinar et al., 2008). The methodology to build the models in both systems will be provided, as well as, the methodology to obtain the atomic parameters, necessary to molecular simulations.
To carry out molecular dynamics studies of polymer systems is necessary to know some important physicochemical properties or thermodynamic parameters of polymers. For the
Molecular Dynamics – Studies of Synthetic and Biological Macromolecules 30
other hand, it is important to know the different methodologies employed to carry out molecular dynamic simulation of polymers.
2. Physicochemical properties of polymers
In this chapter we concéntrate efforts on giving the reader a brief description of some important physicochemical properties of the polymers for molecular simulation analysis analysis. Macromolecular conformation is an important point to consider. The macromolecular chains in dilute solution have variables internal rotational angles, Figure 1. The internal rotational angle can take values that fluctuate within a range so that different minimum energy can be obtained for various values of the angles . The energy difference associated with the variation of this angle is minimal. This leads to a large number of stable conformations and significant mobility to oscillate around these conformations. Both factors cause that the macromolecule has a significant flexibility. Experimentally the dimensional parameters that characterize a macromolecule can only be characterized in terms of statistical parameters that represents an average over all conformations. The end-to-end distance and radius of gyration are statistical parameters that characterize the spatial distribution of a chain macromolecule(Flory, 1969, 1995).
Fig. 1. Three successive bonds for a chain. Where and represents the bond angle and internal rotation angle, respectively.
The end-to-end distance 隼 堅態 伴 represents the distance between end chains. This parameter can vary from a maximum value, where the polymer chain is fully extended to a minimum value corresponding to the sum of the van der Waals radii of the terminal groups, Figure 2.
The end-to-end distance is a statistical parameter that characterizes the spatial distribution of the chains relating the microscopic with macroscopic properties, also allows to relate the hydrodynamic parameters with thermodynamic parameter, and finally allows to obtain information respect to flexibility chain.
Molecular Dynamics Simulation of Synthetic Polymers 31
Fig. 2. End-to-end distance 隼 堅態 伴 representation to a) fully extended chain model, where 隼 堅態 伴 takes a maximum value and b) 隼 堅態 伴 takes a minimum value and correspond to the sum of the van der Waals radii. 隼 堅態 伴 is defined by the equation 1:
隼 堅態 伴噺 完 堅態激岫堅岻穴堅著待 (1) where W(r) is probability distribution function, defined by
豹 激岫堅岻穴堅 噺 な著待 But the chains may adopt different conformational states depending on the characteristics of the chain, features such as substituents and the solvent. For the different conformational states, there are different chains models. Is not intended to provide a thorough review of statistical mechanics of polymer chains(Flory, 1969), but is important to note that the value of 隼 堅態 伴 depends on two main factors, “short-range” and “long-range” factors. For these two factors, different chain models were raised in the past. Short-range factors involved characteristics of the bonds and interaction between neighboring atoms or groups along a chain, this chain correspond to a rotation free model. Hence, 隼 堅態 伴 can be calculated knowing the values of bond angles and bond distances for all the conformations, the value obtained is called dimension mean square of end-to-end distance 極堅態玉墜捗. Take into account factors such as bond angle restrictions and steric hindrance between substituent groups, we can obtain unperturbed dimension 極堅態玉待, and may be expressed by equation 2:
極堅態玉待 噺 購態極堅態玉墜捗 (2) where is the stiffness coefficient or conformational factor. The 極堅態玉待 is so-called “theta condition”.
In long-range factors are involved the interactions between distant segments along the chain, as well as interaction with the solvent. Taking into account that, two distant segments of a chain, cannot occupy the same place at the same time, arise the excluded volume concept. Under effect of these interactions the end-to-end distance to linear chains in dilute solution, may be described by:
Molecular Dynamics – Studies of Synthetic and Biological Macromolecules 32
隼 堅態 伴怠 態斑 噺隼 堅態 伴待怠 態斑 糠 (3) where linear expansion chain factor. In equation 3, the root-mean-square end-to-end distance 隼 堅態 伴怠 態斑 depends of number of segments, temperature and solvent. When >1 them the interaction between solvent and chains are favorable, this means that excluded volume effect is important. Instead, if the interactions between segments and solvent are unfavorable them tend to decrease; this causes folding of the chains to minimize the contact with the solvent. These effects can be balance and them the polymer chain adopts an unperturbed state.
The radius of gyration is the parameter more appropriate to describe the dimensions of a macromolecule. The mean-square radius of gyration 隼 迎直態 伴 represents the mean square of the distance between each atom in the chain and center of mass of the chain and may be defined to following equation 4:
隼 迎直態 伴噺 岫な 券岻 ∑ 隼 堅沈態 伴津怠⁄ (4) where n is the segments numbers of the chain and 隼 堅沈態 伴 represents the mean-square distance of the i-th segment from the center of mass of the chains. Through the random flight model we can express the radius of gyration in terms to mean-square end-to-end distance, indicating their interchangeability. For a freely rotating chain of n segments of length l, the following relationship is established:
隼 迎直態 伴噺 怠滞 隼 堅態 伴噺 津鎮鉄滞 (5) A complete derivation of these equations can be reviewed in various texts of statistical mechanics of polymers(Flory, 1995) (Yamakawa, 2001). We have said that the dimensional parameters are important to know because of their contribution to the characterization of polymers. In addition, these parameters can be calculated both experimentally and theoretically. For example, radius of gyration has been calculated, in several works, from molecular simulation trajectories and compared with the experimental values(Lee et al., 2006; Prosa et al., 2001, 1997).
3. Molecular dynamic simulation of supramolecular structures at the air-water interface
A great interesting in the last year toward to study theoretical of self-assembly of macromolecular systems have been report(D